USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE

 Imogene Boyd
 10 months ago
 Views:
Transcription
1 Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and E. I. Romensky School of Mechanical and Manufacturing Engineering, UNSW, Sydney 05, Australia Sobolev Institute of Mathematics Siberian Division of Russian Academy of Sciences, Novosibirsk , Russia SUMMARY: The aim of the work is to design hierarchical model for description of the dynamic behaviour of unidirectional composite. On the basis of the Maxwelltype viscoelastic model [] a procedure to derive dynamic equations for the composites is proposed. The space arrangement of constituents in the direction transverse to the symmetry axis is out of consideration. In the present paper the bonding between the constituents is assumed to be perfect. Comparing data of the known theories and experiments with the results obtained, the effective elastic characteristics are in good agreement for fibrous composites, and are coincident with the known theory [] for laminated composites. Assuming finite elastic deformations, the procedure gives the equations containing the wellknown plastic spin. The model obtained is applied to the problem of the shockwave propagation in an obliquely loaded laminated composite. The shockwave splitting occurs that is in agreement with the experimental observation [3]. The phenomenon is associated with peculiarities of the loaddeformation curve, which shows the variation of the strength properties of the composite due to the reinforcement rotation during the loading. KEYWORDS: Hierarchical model, homogenization approach, shockwave propagation, offaxis loading, laminated composite. INTRODUCTION Practical needs in the consideration of composite as a homogeneous anisotropic medium gave rise in popularity of homogenization procedures. This consideration provides quite correctly general description of the process of loading. Simple homogenization rules work well in numerous applications and these are very convenient for the finiteelement computations of structures containing composite members. However, in some cases the micromechanical peculiarities are of interest and description of residual stresses and internal microstresses is required. Micromechanical approaches give useful information but these are restricted to the consideration of individual fibre [, 46]. Therefore, the homogenization approach is best suited for an analysis of the composite as a whole. Most of the known procedures aim to derive elastic moduli of composite in order to use the anisotropic theory of elasticity in finite II  55
2 Proceedings of ICCM, Gold Coast, Australia, 4th8th July 997 element computations. Our objective is to design a procedure for derivation of evolution equations. In doing so the effective elastic characteristics are a byproduct. Threelevel hierarchy is established during the application of the procedure. The low level is associated with the microstructural process in the composite's constituents (irreversible processes in the lattice caused by dislocations and microdefects). In the paper this level is realized by the description of the constituents by the Maxwelltype viscoelastic model []. The second level is associated with the micromechanics of the composite and results from the description of the fibrematrix interaction. Finally, the upper level is presented by the description of the composite as a whole (the phenomenological description) within the framework of the conservation laws and constitutive equations; these latter are derived from the basic model (the low level) and the homogenization procedure (the second level). The resultant equations can also be used in the finite element computations. An application of the model to the threepoint bending problem is presented in the proceedings [7]. The Onzager principle, expressing the symmetry of inelastic reactions to the load, is valid for the model. This principle is of fundamental significance for the design of finiteelement algorithm because it enables one to derive the symmetrical stiffness matrix. THE HOMOGENIZATION APPROACH: BRIEF DESCRIPTION Homogenization procedure has to take into consideration a great number of factors. The composite is a very complex structure and the interaction between individual constituents is hard to analyse. Therefore, a certain degree of idealisation is necessary to describe both the composite as a whole and at least the main features of the constituents' interaction. The main problem in the design of the phenomenological theories is to take into consideration as many factors as possible and to make the derivation as simple and utilitarian as possible. As a basis, we take a complex model for the description of the constituents. This gives us some flexibility in manipulation by assumptions for the second level. Because the utility of derivation and thermodynamical correctness of the model are our objectives, we select a simple set of assumptions for the description of the constituents interaction. Due to the presupposed perfect bonding of components the equality of velocities in the fibres and matrix is assumed. The load transfer between the components is quite complex and depends on the length and quality of fibres. Distribution of radial and circumferential stresses around fibre and the interaction of the stress fields among individual fibres and matrix are also nontrivial issues in the micromechanics of composites. Taking as an example the fibrous unidirectional composite, we consider that the following assumptions are absolutely necessary: i) the difference between the constituents stresses in direction of the fibre line can not be neglected; ii) this difference induces internal microstresses acting in the longitudinal direction. For simplification we assume: i) stresses in the transversal direction are distributed uniformly in both composite s components; ii) the mixture rule for stresses in the longitudinal direction is valid. Mathematical representation of the assumptions stated above is: ( ) ( ) σ = σ = σ, ( i, j) (, ) () II  553
3 Volume II: Fatigue, Fracture and Ceramic Matrix Composites Here the x  direction is assumed to be coincident with the fibre direction, the stresses inside ( fibres are σ ) (, inside matrix  σ ), `averaged' stresses of the composite as a whole  σ. Hereafter, the upper indices in parentheses are associated with the number of a composite' s ( constituent (  fibre,  matrix). It is assumed that only the difference between σ ) and ( ) σ can not be neglected. This difference generates internal microstresses determined by ( variable that presents the difference between elastic microstrains ε ) ( and ε ) : ε ( ) ( = ε ). () ( k Connection with the internal microstresses is obvious because microstresses σ ) are related to ( k ) elastic microstrains ε by the Hooke' s law. An interesting peculiarity of this structural parameter is that it is irreducible at elastic deformations of the composite as a whole including the stress release. Therefore, is connected directly with the residual stresses in the composite. ( k ) On the microlevel the longitudinal stress σ is a sum of the longitudinal microstresses σ proportionally to the fibre volume fraction c: ( ) ( ) σ = cσ + ( c) σ (3) Thus, this procedure avoids the fibre arrangement, the component' s bonding and local distributions of the transverse stresses but enables the longitudinal microstresses to be taken into account. Additional hypotheses for elastic microstrains and thermophysical variables (temperature T and specific entropy s ) are: ( ) ( ) ( ) ( ) T = T = T, s = c s + ( c) s, (4) ( ) ( ) ε = ε ε, (5) ε = c ( ε ε ) + ( c)( ε ε ), ( i, j) (, ), (6) ( ) ( ) ( ) ( ) ( k ) here ε  microstrains induced in the constituents by the irreversible processes after the stress release has occurred. The origin of the least obvious hypothesis (5) results from the micromechanical consideration of the loadingunloading cycle of unidirectional composite in the longitudinal direction. A detailed analysis and derivation of (5) have been carried out in [8]. Similar hypotheses are constructed for the unidirectional laminated composite. Introduction of the assumptions for microstrains and temperature gives an opportunity to connect all microstresses, microstrains and corresponding thermophysical characteristics to the macrovariabes. If the equations of dynamic behaviour for each the composite' s components are given, then, using the hypotheses stated above, we can obtain: i) relationships between stresses and strains (including the temperature and entropy); ii) equations of the dynamics of composite. II  554
4 Proceedings of ICCM, Gold Coast, Australia, 4th8th July 997 Detailed derivation for the case of small elastic deformations is stated for the unidirectional fibrous and laminated composites in [8,9]. Generalisation for the case of finite elastic deformations is based on the use of a transformation of a rectangular system associated with fibre into the Cartesian coordinate system. In fact, the transformation is a matrix of the fibre rotation and it determines fibre location in the stress release state. The transformation of the tensor variables (strains, stresses, the structural parameter ) results in the appearance of the plastic spin in the righthand sides, which are responsible for the inelastic behaviour of composite. In general form the system of equations of the model is: da dt uk + a ik = a ikψ kj, x j db dt = θ b, ik kj d dt = λ + θ θ, (7) ik kj ik kj where ψ ~ = α σ ~ + α σ ~ + α σ ~ + β q ~, 33 ψ ~ = α σ ~ + α σ ~ + α σ ~ + β q ~, (8) 3 33 ψ ~ = α σ ~ + α σ ~ + α σ ~ + β q ~, ~ ~ ~ ψ, ~ ~ ~ ~ = α 66 σ λ = β σ + β σ + β σ 33 + γ q, i j here α, β i, γ  the coefficients derived by use of the homogenization procedure from the functions of the Maxwelltype model for the composite s components [9], they depend on the relaxation functions and the stress state in the constituents. The symmetry of coefficients in (8) expresses the fundamental fact  the Onzager symmetry principle. In the system (7) θ are components of a tensor which is responsible for irreversible change in the fibre orientation, it is a given function when the functions ~ ψ are given. The tensor with components b is a tensor of irreversible rotation for fibre, q ~ = E ~, a tildevariable ~ f is a tensor in the rectangular system associated with either the fibre or the normal to lamina, it is expressed ~ through that in the Cartesian system by the standard transformation rule: f = bik f kmbmj. The system (7) is completed by the conservation laws for energy and momentum, and a given dependence of the internal energy E on the strain tensor, structural parameter and entropy.. EFFECTIVE ELASTIC CHARACTERISTICS To illustrate the influence of the fibre content on elastic muduli, the characteristics in this section will be analysed for the case of isothermal deformation. Invoking the procedure of homogenization, the Hooke' s laws for cons tituents yield the stressstrain relations which are typical for the transversely isotropic material: II  555
5 Volume II: Fatigue, Fracture and Ceramic Matrix Composites where σ = C ε + C ε + C ε, 33 σ = C ε + C ε + C ε, (9) 3 33 σ = C ε + C ε + C ε, σ = C ε, i j C = λ + µ + λ λ λ, C =, λ + µ λ + µ λ + µ λ + µ λ + µ C = +, C3 =,. (0) λ + µ µ λ + µ µ C66 = ( C C3 ) = µ, here λ, µ are the Lame coefficients. Expressions in the angle parentheses present the mixture rule K = ck + ( c) K. K = ck + ( c) K. The longitudinal and transverse Young' s moduli E, E, the shear modulus G and the longitudinal and transverse Poisson' s coefficients ν, ν can be easy linked with C : E G [ ] ( ) ( ) ( C C C ) C C C C C C C =, E =, C + C 3 C CC3 C = C, ν =, ν =. () C + C C C C 66 3 It is interesting to note that the procedure applied to the laminated structure gives the elastic moduli which coincide identically with those stated in the popular monography by Christensen []. Therefore, we shall analyse the dependencies of the elastic constants on the fibre content only for the fibrous composite. The wellknown estimates for an efective modulus of the composite K c (K f  the respective elastic modulus of fibres, K m  the elastic modulus of matrix) are the Voigt estimate (the mixture rule) and the Reuss estimate, respectively [5]: K = ck + ( c) K c f m, K = c K + ( c) K, where c  the fibre volume concentration. c f m The longitudinal Young' s modulus E for the composite in most of theories is in very good agreement with the Voigt estimate (the rule of mixture), experiments are in agreement with this rule, too. Our formulae are not an exclusion and they are practically coincident with the II  556
6 linear dependence of the mixture rule. Proceedings of ICCM, Gold Coast, Australia, 4th8th July 997 Fig. : The transversal Young s modulus (a) and the rigidity modulus (b) for the glass/epoxy fibrous composite. Theoretical and experimental dependencies are not so simple for the transversal Young' s modulus E and the rigidity modulus G. The wellknown approximation for the moduli is the Reuss estimate [5]. It is interesting to note that our dependence for the rigidity modulus is exactly the Reuss estimate. Experiments stated in [4] give the moduli (points in Fig. ) for the glass/epoxy composite (elastic constants for fibre and matrix are E = 73. f G Pa, G f = 30. G Pa, ν f = 0., E = 345. m G Pa, G = 8. G Pa, ν = 035 m m. ). Our results (curves according to equations (0), ()) are compared in Fig. with the theory of [4] and the Reuss estimate of the effective moduli. It is seen that the discrepancy between all the theories and experiment is of the same order. Experimental data for the graphite/epoxyresin composite by Goggin [0] are stated by points in Fig.. Elastic data for the constituents are: the type fibre E f = 395 G Pa, ν f = 08. ; the type fibre E f = 30 G Pa, ν f = 08. ; the fibre in the transversal direction: E f = 76. G Pa, ν f = 08. ; the epoxy resin system: E = 39. m G Pa, ν = 033 m.. Fig. a corresponds to the transversal Young' s modulus E, Fig. b  the rigidity modulus G, Figs. c and d  the longitudinal and transversal Poisson' s ratios ν and ν, respectively. Curves,, 3 in Fig. a correspond to the three types of fibres mentioned above according to the formulae (0), (), curve in Figs. bd  to the fibre type calculated by the same formulae. The data by Goggin [0] have quite large scatter, especially for the Poisson' s ratio. The Young' s modulus of the fibre type is less than that of the fibre type. However, the transverse Young' s modulus of the composite with the fibre type is higher than that with the fibre type (Fig. a). Apparently, this feature is associated with the strong anisotropic properties of fibres. Our model of the constituents is an isotropic material. Therefore, we calculated curve 3 in Fig. a for a fibre with the Youngs s modulus corresponding to the experimental transversal Young s modulus of the graphite fibre. Among theoretical data the wellknown formulae are those by R. Hill [5]. For the constants from (0) they take the form: ( λ λ ) ( λ λ )( λ + µ λ µ ) C c c M C c c = λ + µ ( ), = λ ( ), λ + µ + λ + µ + M II  557
7 Volume II: Fatigue, Fracture and Ceramic Matrix Composites ( µ µ ) C66 = ( C C3 ) = µ c ( c), () µ + M ( ) ( λ + µ λ µ ) C + C3 = λ + µ c ( c), λ + µ + M here f = ( c) f + cf. It is easy to check that at M = 0 these formulae reduce to dependencies (0). Because M has the meaning of the shear modulus we take as an example M = µ. Calculations according to () give the curve 4 in Fig., (a) and curves 3 in Fig., (cd). The semiempirical dependencies by C.Chamis stated in [6] are the curve 5 in Fig. a and curves in Fig. bd. Our formulae describe experiments on the Poisson s ratio in the best way among theoretical data mentioned above. For the transversal Young s modulus and the rigidity modulus the discrepancy between all the theories and experiment is again of the same order. Fig. : The effective elastic characteristics for the graphite/epoxy composite. The transversal Young s modulus (a) (points are the experiments [0]); the rigidity modulus (b); the longitudinal Poisson s ratio (c); the transversal Poisson s ratio (d). The above comparison gives us confidence in the use of the homogenization approach for the derivation of dynamic equations. THE SHOCK WAVE RESPONSE OF COMPOSITE To illustrate the potential of the model a computation of the shock wave propagation in obliquely oriented laminated composite has been conducted. The method of calculation of the system (7) is the finitedifference Godunov scheme widely used for calculations of the shockwaves in gases. The composite structure has been chosen in accordance with an experimental II  558
8 Proceedings of ICCM, Gold Coast, Australia, 4th8th July 997 sample by Sve and Okubo [3], where the Al/Lexan composite has been oriented symmetrically (Fig. 3a) and obliquely (Fig. 3b) to the shock wave. Fig. 3: Sketches for the straightward and obliquie shockwave loading of the laminated composite. In order to understand the process of the offaxis loading let us consider the loading of the representative volume of the composite by uniaxial stress. The sketch of the process is drawn in Fig. 4. The corresponding loaddeformation curve computed by the model shows that in certain range of orientations the stress response is complex due to rearrangement of the composite structure during the loading. At the symmetrical loadings (the cases and 3) the composite strengths correspond to those of the fibre or matrix. For the offaxis loading (the case ) the composite strength changes during the deformation, depending on the reinforcement direction. Fig. 4: Schemes of the offaxis loading and calculation of the loaddeformation curve for the case of rotation of the reinforcement. Coefficients α, β, γ of the functions ψ in (8) which are responsible for the inelastic II  559
9 Volume II: Fatigue, Fracture and Ceramic Matrix Composites limit on the strain rate. The method for the construction of the functions can be found in []. Fig. 5: Calculation of the shockwave response of the symmetryoriented and obliquely oriented laminated composite;  the velocity profile,  the microstress profile, 3  the change in the fibre orientation. The shockwave propagation calculated for the samples in Fig. 3 has a number of peculiarities. At symmetrical loading (velocity versus coordinate in the sample at a moment of time  the curve, Fig. 5a), the fibre orientation does not change during the process (curve 3), ~ (curve ) associated with the internal microstress (the difference in elastic strains between the constituents) changes only after the elastic wave has passed and the plastic wave has induced the microstress in the sample. However, in the case of offaxis loading (the orientation angle ϕ 0 = 47 ) the fibre orientation becomes an essential factor due to the rearrangement stated in Fig. 4. Initially, the elastic wave acts as in the preceding case (velocity  curve in Fig. 5b), then the successive load changes the layer orienation and modifies the strength properties of the sample. It is seen from Fig. 5b that in the second wave the angle orientation has been changed (curve 3), a rise in ~ (curve ) indicates that the composite in these points is out of elastic range and the change is associated with the structural rearrangement. The third wave performs the final loading up to the limit determined by the striker. Fig. 6: Comparison between the calculated (curve ) and the experimental [3] (curve ) velocity profiles. The comparison of the calculation with the experiments [3] shows good agreement between the velocity profiles (Fig. 6). II  560
10 Proceedings of ICCM, Gold Coast, Australia, 4th8th July 997 CONCLUSION A homogenization procedure for unidirectional composite is proposed in the paper. The aim of the approach is to design a threelevel hierarchical model for description of the dynamic behaviour of the composite materials. Effective elastic characteristics obtained by the procedure for the fibrous and laminated composite are within the range of the wellknown theoretical and experimental data. The model is suitable for description of the shockwave data for composites. The calculation of the obliquely loaded composite is in good agreement with the known experiment [3]. REFERENCES. Godunov, S.K. and Romensky, E.I., "Nonstationary Equations of Theory of Nonlinear Elasticity in the Eulerian Coordinates", Prikl. Mekh. i Tekh. Fiz. [Engl. transl. Appl. Mech. Techn. Phys.], Vol. 3, No. 6, 97, pp Christensen, R.M., Mechanics of Composite Materials, John Wiley, New York, Sve, C. and Okubo S., "Experiments on Pulse Propagation in an Obliquely Laminated Composite", Journal of Applied Mechanics, Vol. 39, 974, pp Tsai, S.W. and Hahn, H.T., Introduction to composite materials, Technomic Pub., Westport, Hill, R., Theory of Mechanical Properties of Fibre Strengthened Materials, J. Mechanics and Physics of Solids, Vol., 964, pp Chawla, K.K., Composite Materials, SpringerVerlag, New York, Resnyansky, A.D., Simulation of Flexure in Off axis ThreePoint Bending Test by a FiniteElement Code, The Present Proceedings. 8. Resnyansky, A.D. and Romensky, E.I., "Model of Viscoelastic Unidirectional Composite with Coupled Thermal and Elastic processes", Proceedings 9th International Symposium on Shock Waves, Marseille, France, July 630, 993, Vol. III: Shock Waves in Condensed Matter and Heterogeneous Media, Brun, R., Dumitrescu, L.Z., Eds, pp Resnyansky, A.D. and Romensky, E.I., "Model of Dynamic Deformation of a Laminated Thermoviscoelastic Composite", Combustion, Explosion, and Shock Waves (Fizika Gorenia i Vzryva), Vol. 9, No. 4, 993, pp Goggin, P.R., The Elastic Constants of CarbonFibre Composites, Journal of Materials Science, Vol. 8, 973, pp Resnyansky, A.D. and Merzhievsky, L.A. "On Determination of Parametres of Dependence of The ShearStressRelaxation Time", [In Russian], Fizika Gorenia i Vzryva, Vol. 8, No. 3, 99, pp II  56
Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationThe Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials under Kinematic Harmonic Loading
Mechanics and Mechanical Engineering Vol. 21, No. 1 (2017) 157 170 c Lodz University of Technology The Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationConstitutive models: Incremental (Hypoelastic) Stress Strain relations. and
Constitutive models: Incremental (Hypoelastic) Stress Strain relations Example 5: an incremental relation based on hyperelasticity strain energy density function and 14.11.2007 1 Constitutive models:
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationStresses and Strains in flexible Pavements
Stresses and Strains in flexible Pavements Multi Layered Elastic System Assumptions in Multi Layered Elastic Systems The material properties of each layer are homogeneous property at point A i is the same
More informationIn this section, thermoelasticity is considered. By definition, the constitutive relations for Gradθ. This general case
Section.. Thermoelasticity In this section, thermoelasticity is considered. By definition, the constitutive relations for F, θ, Gradθ. This general case such a material depend only on the set of field
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationMULTISCALE MODELING OF TRIAXIAL WOVEN FABRICS. APPLICATION TO SATELLITE ANTENNA
MULTISCALE MODELING OF TRIAXIAL WOVEN FABRICS. APPLICATION TO SATELLITE ANTENNA JEANSEBASTIEN GERARD 1, STEPHANE CATALAO 2, ROGER ASSAKER 2, JULIAN SANTIAGO PROWALD 3 1 exstream engineering SA, Rue
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationSTRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLASFIR
UNITED STATES DEPARTMENT OF AGRICULTURE. FOREST SERVICE  FOREST PRODUCTS LABORATORY  MADISON, WIS. STRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLASFIR NOVEMBER 1963 FPL020 STRESSES WITHIN CURVED LAMINATED
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationLinear Cosserat elasticity, conformal curvature and bounded stiffness
1 Linear Cosserat elasticity, conformal curvature and bounded stiffness Patrizio Neff, Jena Jeong Chair of Nonlinear Analysis & Modelling, Uni Dui.Essen Ecole Speciale des Travaux Publics, Cachan, Paris
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationA NEW REFINED THEORY OF PLATES WITH TRANSVERSE SHEAR DEFORMATION FOR MODERATELY THICK AND THICK PLATES
A NEW REFINED THEORY OF PLATES WITH TRANSVERSE SHEAR DEFORMATION FOR MODERATELY THICK AND THICK PLATES J.M. MARTÍNEZ VALLE Mechanics Department, EPS; Leonardo da Vinci Building, Rabanales Campus, Cordoba
More informationThermoMechanical Response of Functionally Graded Materials for Extreme Environments
ThermoMechanical Response of Functionally Graded Materials for Extreme Environments Introduction In recent years, functionally graded materials (FGMs) have attracted much interest in a wide range of engineering
More informationComputational Biomechanics Lecture 2: Basic Mechanics 2. Ulli Simon, Frank Niemeyer, Martin Pietsch
Computational Biomechanics 016 Lecture : Basic Mechanics Ulli Simon, Frank Niemeyer, Martin Pietsch Scientific Computing Centre Ulm, UZWR Ulm University Contents .7 Static Equilibrium Important: Freebody
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationMaterial parameters for electrostriction
Material parameters for electrostriction Yuri M. Shkel and Daniel J. Klingenberg a) Department of Chemical Engineering and Rheology Research Center, University of Wisconsin, Madison, Wisconsin 53706 Received
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationHooke s law and its consequences 1
AOE 354 Hooke s law and its consequences Historically, the notion of elasticity was first announced in 676 by Robert Hooke (635 73) in the form of an anagram, ceiinosssttuv. He explained it in 678 as Ut
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationProceedings of the ASME th International Conference on Ocean, Offshore and Arctic Engineering OMAE2016 June 1924, 2016, Busan, South Korea
Proceedings of the ASME 26 35th International Conference on Ocean, Offshore and Arctic Engineering OMAE26 June 924, 26, Busan, South Korea OMAE2654554 LOCAL STRAIN AND STRESS CALCULATION METHODS OF IRREGULAR
More informationTensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites
Tensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites Journal of Reinforced Plastics and Composites, Vol. 9 (March, 1990) pp. 127133 W. H. PROSSER NASA Langley Research Center
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationA multiscale approach for composite materials as multifield continua
Materials Science Forum Vols. 539543 (27) pp. 25512556 online at http://www.scientific.net (27) Trans Tech Publications, Switzerland A multiscale approach for composite materials as multifield continua
More informationDegree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann
Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017 DEGREE THESIS Arcada University of Applied Sciences, Helsinki,
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationGame Physics. Game and Media Technology Master Program  Utrecht University. Dr. Nicolas Pronost
Game and Media Technology Master Program  Utrecht University Dr. Nicolas Pronost Soft body physics Soft bodies In reality, objects are not purely rigid for some it is a good approximation but if you hit
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationNumerical modelling of elasticplastic deformation at crack tips in composite material under stress wave loading
JOURNAL DE PHYSIQUE IV Colloque C8, supplément au Journal de Physique III, Volume 4, septembre 1994 C853 Numerical modelling of elasticplastic deformation at crack tips in composite material under stress
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationMechanics of Solids notes
Mechanics of Solids notes 1 UNIT II Pure Bending Loading restrictions: As we are aware of the fact internal reactions developed on any crosssection of a beam may consists of a resultant normal force,
More information